Inﬂuence of electrical operating conditions and active layer thickness
on electroluminescence degradation in polyﬂuorene–phenylene
based light emitting diodes
, B. Arredondoa
, A.L. Alvareza
, R. Mallaviab
, A. Salinasb
, X. Quintanac
, J.M. Otónc
aDpto. Tecnología Electrónica, Universidad Rey Juan Carlos, C/Tulipán s/n, 28933 Móstoles, Madrid, Spain
bInstituto de Biología Molecular y Cellular, Universidad Miguel Hernández, Av. del Ferrocarril, s/n Elche 03202 Alicante, Spain c
Dpto. Tecnología Fotónica, Universidad Politécnica de Madrid, Ciudad Universitaria s/n, 28040 Madrid, Spain
a r t i c l e
i n f o
Received 14 July 2008
Received in revised form 13 November 2008 Accepted 16 November 2008
Available online 1 January 2009 The review of this paper was arranged by Dr. Y. Kuk
Polymer light emitting diodes Degradation
a b s t r a c t
We have studied the inﬂuence of the electrical working conditions (voltage or current biased), and the active layer thickness on electroluminescence (EL) properties of polymeric light emitting diodes based on poly-[9,9-bis(60-cyanohexyl)-2,7-ﬂuorene-alt-co-1,4-phenylene], [PFP:(CN)
2]. Diodes with different active layer thicknesses (55–140 nm) have been fabricated and characterized. Temporal evolution of the spectra at constant bias and current, as well as the spectral evolution with the current, has been per-formed. Excitation photoluminescence has been used to discriminate between intrinsic and defect-related transitions. The relative spectral area arising from defects has been quantiﬁed by means of Gauss-ian deconvolution for different device excitations. Active layer thickness has been observed to play an important role on the emissive spectral shape. In thick samples EL tends to resemble ﬂuorescence from the pristine material. In contrast, thinner samples clearly show two additional bands related to defects: the ﬁrst one is structured in the range 470–510 nm, which is proposed to be due to electron accumulation in the active layer, and a second band at 535 nm, arising from on-chain keto defects due to the presence of oxygen. The role of the electron blocking character of the PEDOT:PSS on the spectral shape, as well as the inﬂuence of the active layer thickness on the oxygen concentration, are discussed.
Ó2008 Elsevier Ltd. All rights reserved.
Since the discovery of polyﬂuorenes (PFs), they have drawn great attention due to their interesting properties as blue emitters for solution-processable polymer light emitting diodes (PLEDs): high efﬁciencies, reasonable mobilities and good thermal and chemical stability. Besides, the solubility and processability of these polymers can be easily improved, by substituting the C-9 car-bon, without signiﬁcantly increasing the steric interactions in the polymer backbone, which eventually confers them better perfor-mance than other approximations for blue emission using poly-paraphenylene (PPP).
Despite PF and copolymers being promising candidates as blue emitting materials, most of the synthesised derivatives have so far a problem related to colour instability, consisting of the develop-ment of undesired low energy emission bands during device oper-ation. This has been attributed to a variety of degradation processes, and eventually means a loss of colour saturation. As a result, PFs degradation is currently the main drawback when using
these materials as active layers, and consequently, this issue is being the subject of numerous studies[2,3].
Typical blue emission of PF based diodes is dominated by highly efﬁcient intrinsic bands corresponding to the excitonic transition, and a noticeable vibronic splitting up to several orders. Particular interest received an extrinsic green emission band at 530 nm. This band appears after thermal annealing of the polymer ﬁlm or during device operation, both in air. The initial hypothesis attributed this phenomenon to intermolecular excimer formation between poly-ﬂuorene chains[4,5]. Recent experimental evidences have estab-lished that the origin of the green emission is related to the presence of ﬂuorenone defects (C@O bonds at the C-9 carbon) in the polymer chain upon thermal or photo-oxidation in the pres-ence of oxygen[6,7]. The relevance of this defect is due to its efﬁ-ciency as emissive centre, favouring the energy transfer from the fundamental excitonic level. Zhao et al. associated the green band to the formation of an insoluble, cross-linked species that is formed upon thermal degradation and may be enhanced by annealing at high temperatures. Other authors have suggested that ﬂuore-none defects are originated during device processing. In particular, the deposition of low work function metals such as Ca or Ba n-dopes the polymer, and the doped polymer is oxidized during
0038-1101/$ - see front matterÓ2008 Elsevier Ltd. All rights reserved. doi:10.1016/j.sse.2008.11.005
* Corresponding author. Tel.: +34 (91) 488 7178; fax: +34 (91) 664 7494.
E-mail address:email@example.com(B. Romero).
Contents lists available atScienceDirect
device fabrication generating ﬂuorenone defects and thus the appearance of the green band.
In addition, another extrinsic band with structure in the range 470–515 nm, has been observed in many PLEDs. Although several authors have detected this structure[8–14]only a few have pro-posed hypothesis related to its nature. The origin of this peak is still unclear and is subjected to controversy. Gamerith et al. identiﬁed for ﬁrst time this band as being independent on the ﬂuorenone de-fect. They suggested that it may feature more than one peak, and proposed that it is due to chemical interaction in the presence of oxygen between the polymer and an easily oxidized cathode metal (Ca, Al), although the authors could not determined the exact nat-ure of these interfacial defects. Recently, based on in situ pho-toluminescence (PL) measurements during cyclic voltammetry in an oxygen-free environment, Montilla et al. proposed that this spectral feature is related to the electrochemical degradation of the polymer, which would generate the appearance of a new cross-linked species that was isolated and analyzed. This reac-tion does not take place during oxidareac-tion (hole injecreac-tion) but spe-ciﬁcally in the presence of an excess of electrons above a critical value, regardless the presence of oxygen.
The goal of this work is to thoroughly study the feature at 470– 515 nm in polyﬂuorene–phenylene-based diodes with different ac-tive layer thickness. To do so, we have developed PLED matrix, based on this promising material as active layer. Synthesis and fab-rication details are explained in Section2. The polymer used is a new derivative of poly(2,7-ﬂuorene-alt-co-1,4-phenylidene) (PFP), which presents a cyanide group as a ﬁnal functional group of the hexyl chain at the C9-position of the ﬂuorene ring, (PFP:(CN)2).
Diodes with different active layer thickness, ranging from 55 nm up to 180 nm, have been fabricated, in air or inert atmo-sphere. Characterization results are provided in Sections3 and 4. Electroluminescence (EL) was characterized under diverse bias conditions, observing different patterns when changing the active layer thickness. Emission and excitation PL spectra have been re-corded inside and outside diodes in order to identify different chemical species. We have also used the analysis of Gaussian deconvolution to obtain quantitative information on defects as evolving with operational conditions. Eventually, in Section 5, two different mechanisms are proposed and discussed in order to explain spectral changes: on one hand, the accumulation of elec-trons favoured by the slight blocking character of the PEDOT:PSS interface is sensitive to the active layer thickness, and may in turn modify the recombination zone. On the other hand, it is considered that the remained oxygen concentration inside the sample de-creases when increasing the active layer thickness.
2. Fabrication procedure
Indium tin oxide (ITO) was used as anode and Poly(3,4-ethyl-enedioxythiophene)/poly(4-styrenesulfonate) (PEDOT:PSS) was used as hole injection layer, in order to improve the electrical per-formance. The ﬁnal device structure is ITO/PEDOT:PSS/PFP:(CN)2/ Al.
Device fabrication includes three steps: synthesis of the new material, thin ﬁlm preparation (thickness calibration), and device processing. Every step is described below.
(Fig. 1) was synthesized via a Suzuki coupling reaction using
1,4-phenyldiboronic acid and 2,7-dibromo-9,9-bis(60-cyano)ﬂuorene with high yield . The batch of the polymer has an average
molecular weight of MW= 5.6104g/mol, corresponding to around 100 monomer units per polymer chain, and the index poly-dispersity was 1.95. The introduction of the phenylene group in the conjugated chain results in a 0.2 eV lowering of the LUMO with re-spect to the typical value in PFs, which enables easier electron injection.
2.2. Solution and thin ﬁlm preparation
It is well known that spin-casted ﬁlm thickness is mainly inﬂu-enced by the solution concentration. Solutions in tetrahydrofurane (THF) were heated (just below the boiling point) and introduced in an ultrasonic bath during 1 h in order to improve the solubility of the polymer in the solvent. Subsequently, they were ﬁltered through a 0.45
lm ﬁlter before being spin-casted at 6000 rpmdur-ing 30 s onto a glass substrate. Finally they were annealed at 80°C during 30 min.
Film thickness was determined using an Alpha-Step 200 contact proﬁlometer.
2.3. LED fabrication
The entire fabrication process is carried out in a clean room (class 10,000). Commercial indium–tin-oxide (ITO, thick-ness = 100 ± 5 nm) coated glass is used as substrate. Prior to ﬁlm deposition, the substrates went through a typical organic material cleaning process. The ﬁnal diode passive matrix contains eight diodes with two different radii, 0.5 and 0.75 mm, consisting of a common cathode, aluminium (Al), and an ITO anode.
The fabrication process consists of several steps. The ITO coated glass is patterned by means of a photolithographic process. In a second photolithographic process, wells in the photoresist are dug on top of ITO pads. The insulating behaviour of the photoresist avoids leakage currents between adjacent diodes. Next, a hole transport layer, poly(3,4-ethylenedioxythiophene)/poly(4-styrene-sulfonate) (PEDOT/PSS), is spin-casted at 6000 rpm and dried at 110°C for 30 min. Such material is insoluble in organic solvents and therefore prevents the photoresist to be dissolved by the sol-vent of the active polymer. The organic active layer, a solution of PFP:(CN)2 in THF, is spin-casted at 6000 rpm and annealed at 80°C for 30 min. The Al cathode is thermally evaporated on top of the organic layer surface in an atmosphere of 106Torr.Fig. 2a shows the layer structure. Devices are encapsulated using a glass cover attached by a bead of epoxy adhesive. This process is carried out in a glove box under N2atmosphere. Finally, contact wires are indium soldered. The ﬁnal device is the eight diode passive matrix shown inFig. 2b. Biasing is provided through an ITO path that con-nects each contact to the outer wire.
3. Electrical and optical characterization
Current–voltage (I–V) characteristics were recorded using an Agilent 4155C semiconductor parameter analyzer and an Agilent
41501B SMU pulse generator. The samples were pulsed biased. The pulse width was set to 0.5 ms and the duty cycle was 0.5%, in order to minimize device degradation.
EL spectra were recorded using a CS-1000 Minolta Spectroradi-ometer. Samples were voltage driven with a pulse train with the same pulse width and duty cycle used in the electrical measure-ments (0.5%).
Steady-state emission and excitation spectra were acquired at room temperature using a PTI QuantaMaster Model QM-62003SE spectroﬂuorimeter for different devices using a solid support well-adjusted (or aligned) light beams.
4.1. Electrical behaviour
Fig. 3shows the current density–voltage (J–V) for devices with
different active layer thicknesses, ranging from 55 nm to 180 nm. As was expected, threshold voltage increases with active layer thickness, but not only due to the limiting effect of the bulk cur-rent, but also due to a decrease of the injection rate, associated to a reduction of the internal electric ﬁeld at the interface.
Although the best device, in terms of lowest threshold voltage is the thinnest one, we have checked that the probability of having short circuits increases when the active layer thickness goes below 40 nm, in agreement with. In our case, devices with active lay-ers of 55 nm show even better success probability, in terms of opti-cal lifetime, than those with a thicker active layer.
4.2. Optical behaviour
InFig. 4, emission and excitation PLs (recorded at 420, 444 and
470 nm) have been performed in a pristine 55 nm layer. The emis-sion PL curve shows one peak at 420 nm corresponding to the
excitonic transition, as well as two features at 444 and 470 nm. The ﬁrst one is typically attributed to the ﬁrst vibronic peak, and the latter is tentatively assigned to a second order vibronic replica, supported by the coincidence in the energy shift (around 155 meV). The fact that no signiﬁcant differences have been found in the excitation PL measurements at these wavelengths indicates that the optical response arises from the same intrinsic material and supports the previous assumption. Attending to this, three Gaussian curves will be used in this range when decomposing EL measurements, in order to take into account every intrinsic transition.
Fig. 5shows two different EL spectra recorded from identical
structural devices (around 55 nm active layer thickness). The only difference in the fabrication process took place during the active layer annealing: while sample (a) was cured in N2 atmosphere, sample (b) was cured in air atmosphere. The shorter wavelength region is dominated by two well resolved peaks at 423 nm and at
Glass substrate ITO
Active Layer Aluminium
Fig. 2.(a) Layer structure of the fabricated devices. (b) PLED passive matrix.
0 5 10 15 20 25 30 35 40
0.00 0.05 0.10 0.15 0.20 0.25 0.30 0.35
L= 55nm L = 95 nm L = 140 nm L = 180 nm
Fig. 3.J–V characteristics of PFP:(CN)2based diodes with different active layer
300 350 400 450 500 550 600
0.0 0.2 0.4 0.6 0.8 1.0
Excitation PL at 470 nm Excitation PL at 420 nm Excitation PL at 444 nm
Fig. 4.Normalized emission and excitation PL at 420, 444 and 470 nm for a 55 nm PFP:(CN)2layer.
400 500 600
0.0 0.2 0.4 0.6 0.8 1.0
Wavelength (nm) (a) (b)
445 nm, corresponding to the excitonic and ﬁrst order vibronic transitions, respectively. A well known broad band centred at 535 nm is observed in the air-cured sample (open circles), while this feature is less pronounced in the N2dried sample (solid cir-cles). As explained above, this is in agreement with the theory that attributes this band to the incorporation of oxygen as C'O bonds in the polymer backbone, during the fabrication process.
It is worth noticing the appearance of an additional feature at around 470 nm in both spectra, which, despite matching the wave-length of the second order vibronic replica, shows an excessive intensity in the absence of oxygen. In order to thoroughly study these defect-related bands, three different experiments have been designed: in (a) EL spectra were recorded at a constant voltage dur-ing several hours of operation, in order to study the temporal evo-lution of the electrical response and the spectral shape (b) EL spectra were recorded applying a constant current, which will help to discriminate between pure electrical and electro-optical degra-dation. (c) EL spectra were recorded increasing the bias current.
4.2.1. Spectral evolution at a constant voltage
EL spectra were recorded at a constant voltage during several hours of operation, in order to study the temporal evolution of the electrical response and the spectral shape.Fig. 6a shows the evolution of the EL recorded from a thick (140 nm) active layer diode, along 6 h of operation. The bias voltage was set to 24.4 V, just above the onset for EL (notice that active layer thickness is 140 nm). As can be observed, the spectra are mainly composed by the excitonic band centred at 423 nm, a vibronic shoulder at 445 nm, and a second vibronic replica at around 470 nm. Bands associated to the previously mentioned defects (from 470 nm to 530 nm) are hardly observed in these spectra. Apparently, thicker samples seem to be less affected by extrinsic factors such as
elec-tron accumulation, oxygen and moisture. This will be discussed in Section5.
The total luminance decayed at a half of the initial value after 3 h of operation (Fig. 6b), but no changes in the spectral shape are observed, except for a smooth broad band at 590 nm. By mon-itoring the device current, it has been checked that the decrease of the luminance is due to a proportional current reduction. This is not accompanied by signiﬁcant changes in the spectral shape and thus is identiﬁed only as pure electrical degradation. This effect may be attributed to a loss of ohmic injection at the polymer/PED-OT:PSS interface (stressing). Recent investigations have dem-onstrated that trapped water in the organic layers (PEDOT:PSS is an emulsion in water) is a major source of electrical instability
EL spectra were recorded applying a constant current, adjusting the voltage level in time, which will help to discriminate between pure electrical and electro-optical degradation.Fig. 7a shows the evolution of the EL from a thin (55 nm) active layer diode, along al-most 3 h of operation, setting the bias current to 4.3 mA. Mathe-matical decomposition, assuming Gaussian shapes for the energy transitions, has been performed. It should be pointed out that, although spectra are plotted as function of wavelength, Gaussian deconvolution was performed in the energy domain. Generally, the pristine EL spectra can be reasonably well described by three intrinsic peaks at 420 nm (excitonic), 445 nm (ﬁrst vibronic) and 470 nm (second vibronic) while degraded spectra need the contri-bution of two additional extrinsic peaks that account for the struc-tured electro-optical degradation band  as well as the ﬂuorenone band. Attempts to include other additional Gaussians in this spectral region were discarded since they did not lead to a
400 500 600
0.0 5.0x10-6 1.0x10-5 1.5x10-5 2.0x10-5
First EL recorded
After emitting 2 hours
After emitting 4 hours
After emitting 6 hours
0 1 2 3 4 5 6
0 2 4 6 8 10 12 14 16
Fig. 6.(a) EL spectra evolution for a 140 nm sample during 6 h and (b) luminance (cd/m2
) vs. time of operation at a constant voltage (24.4 V).
400 450 500 550 600 650
0.0 1.0x10-5 2.0x10-5 3.0x10-5 4.0x10-5 5.0x10-5
After emitting 3 hours
Wavelength (nm) J = 550 mA/cm2 After emitting 1 hour
20 40 60 80 100 120 140 160 180
60 80 100 120 140 160 180 200
Fig. 7.(a) EL spectra evolution for a 55 nm sample driven at a constant current density (550 mA/cm2) during 3 h. Spectra are recorded every 20 min. Gaussian
unique solution.Fig. 7a shows this decomposition for the last spec-trum (dashed lines) showing that the apparent height increase of the vibronic peak at 445 nm is mainly due to the inﬂuence of the extrinsic feature at 470 nm. In fact, the vibronic/excitonic intensity ratio holds rather constant along time.
After several hours of operation, it may be noticed that the shoulder at 470 nm enhances, similarly as observed when an ex-cess of electron concentration remains inside the active layer
. In fact, after 3 h of operation, the intensity of this shoulder al-most reaches that of the excitonic peak. For this reason, the excita-tion PL at different wavelengths (420, 470 and 538 nm) have been performed over a degraded diode (55 nm thick). In contrast to the results obtained in a pristine material, a slight difference between the excitation PL recorded at 470 nm (dotted) and that at 420 nm (the intrinsic emission, dashed) is found, supporting the hypothesis of the existence of a new chemical species. This difference becomes stronger for the excitation PL recorded at longer wavelengths such as 538 nm (seeFig. 8).
Also, we observed that the luminance is kept cuasi-constant along time (seeFig. 7b).
4.2.2. Spectra evolution with current injection level
EL spectra were recorded increasing the bias current in order to clarify the study of each transition separately. This experiment, which implies a severe degradation, has been carried out in three different samples: (i) air-cured thin samples (55 nm), (ii) N2cured thin samples (55 nm) and (iii) N2cured thick samples (140 nm).
Fig. 9shows the normalized EL spectra, together with its
Gauss-ian deconvolution, for a 55 nm sample cured under air atmosphere at two different injection bias levels. As can be observed, the inten-sity associated with the 470 nm Gaussian has been promoted by increasing injection level.
For the 55 nm sample cured in N2, current density was varied from 40 mA/cm2up to 1400 mA/cm2.Fig. 10a–c shows the normal-ized spectra, together with their Gaussian deconvolutions, for three different current density levels: 40 mA/cm2, 400 mA/cm2, and 1400 mA/cm2. A quick look at the EL reveals that the relative con-tribution of the defect structured band (from 470 to 510 nm) in-creases with current. The Gaussian deconvolution conﬁrms this fact, as is shown inFig. 10d, where the sum of the relative spectral area of the defect bands is plotted vs. current density. Notice that the greatest changes take place at initial currents, and eventually tend to saturation, when most of the material is already degraded.
Fig. 11shows EL of the 140 nm sample, cured under identical
conditions as the 55 nm sample, for different current density lev-els. The spectra, when compared to previous ones, clearly show that the studied defect bands are much less pronounced in thicker
samples than in thinner ones, even when the increase of carrier density is one order of magnitude. Instead, a new broad band cen-tred at around 590 nm emerges, which is correlated to material damage upon optical inspection of the device. This will be dis-cussed in next section.
Previous results pose several questions that will be discussed below. The ﬁrst one is related to the changes of the EL spectral shape with the active layer thickness. The second one concerns the appearance of the electrooxidation feature between 470 and 510 nm with increasing bias current.
Majority carriers (holes) are injected from the metal contact into the bulk by a jumping process in which the interface electric ﬁeld helps to overcome the injection barrier between the tandem (ITO/PEDOT:PSS) and the active layer . Holes are then trans-ported mainly by hopping along the bulk, and those that do not recombine or accumulate as space charge, are evacuated through the cathode. This means that, at a certain time, the steady current generates a residual (generally small, for the high energy barriers considered) hole density inside the device that depends on the mobility value. In contrast, the scenario for transport of minority carriers (electrons) is very different. At a sufﬁcient high voltage, they are injected from the cathode (Al) into the active layer. Elec-trons are transported along the active layer (PFP) and those that do not recombine reach the PEDOT:PSS and presumably accumulate due to its relative good electron blocking properties . The blocking character is not only favoured by the interface barrier (le-vel alignment) but also by a reduction of carrier mobility in the PEDOT: PSS. In this sense, the negative ionic character of the PSS is expected to block the electron path.
In the case of thin samples, electrons have to cover a small dis-tance before reaching the PEDOT:PSS, reducing the probability that an electron recombines in the PFP layer, and then favouring an accumulation due to the PEDOT:PSS interface. This may shift the recombination zone towards that interface, as observed in multi-layer structures. Eventually, the electron density increase will enhance the degradation mechanisms, promoting the 470 nm peak in the EL spectra. This is supported by cyclic voltammetry studies that reveal that the 470 nm peak arises from new chemical species that appear as a result of an excess of electrons. On the con-trary, increasing the active layer thickness raises the probability that an electron recombines in the PFP layer, lowering the electron
300 350 400 450 500 550 600
0.0 0.2 0.4 0.6 0.8 1.0
Wavelength (nm) PL
Excitation PL at 420 nm Excitation PL at 470 nm Excitation PL at 538 nm
Fig. 8.Normalized emission and excitation PL (at 420, 470 and 538 nm) for a 55 nm PFP:(CN)2degraded diode.
400 500 600 700
0.0 0.2 0.4 0.6 0.8 1.0 0.0 0.2 0.4 0.6 0.8 1.0
16 V 13 V
accumulation effect due to the PEDOT interface, and thus, dimin-ishing degradation and extrinsic peaks in the EL spectra.
On the other hand, it has been mentioned the reactivity of poly-ﬂuorene derivatives in the presence of oxygen. Many studies have proven the formation of the ﬂuorenone upon reaction with the C-9 carbon, resulting in an emissive band centred at 530 nm. In this context, it seems interesting to study the inﬂuence of the active layer thickness on this degradation mechanism. To the best of our knowledge, no research has been performed to study the oxy-gen diffusion length in polyﬂuorene layers. Few studies on the incorporation of oxygen via creation of free radicals in polymers such as PMMA and PVA reveal diffusion coefﬁcients of the order of 1012m2/s, which guarantee fast oxygen diffusion in these materials. In fact, the average diffusion distance,hdi, scales with diffusion coefﬁcient, D, and time, t, as hdi ¼pﬃﬃﬃﬃﬃﬃDt, (according to the Flick’s Law), resulting in a diffusion distance of 1
lm in 1 s ofexposure. In this context, Gammerith et al. performed an in situ PL study during thermal polyﬂuorene oxidation, and observed that
changes due to creation of defects took place in a few seconds. Regardless the oxygen diffusion length in polyﬂuorenes, a thick-ness increase of the active layer decreases the effect of oxygen in the polymer, as may be concluded from two considerations:
(a) In the case the oxygen diffuses along the entire layer, a thicker sample would contain a lower oxygen concentration for the same exposure time.
(b) In the case the oxygen diffuses up to a distance close to the cathode, a thickness increase of the active layer favours that most of the recombination takes place far from that region.
The second remaining question is why the electroxidation fea-ture at 470 nm is less pronounced in thick samples despite increas-ing bias current.
In the same framework of the previous explanations, it may be proposed that for thick devices, and even in the case of high bias currents, the probability of an electron to recombine inside the ac-tive layer is higher than in thinner samples, diminishing the risk of accumulation at any interface, and thus, reducing the appearance of the electrooxidation peak in the EL spectra.
In practice, the determination of the active layer thickness is a critical issue when designing an OLED. Previous observations sug-gest that thick active layers, above 100 nm, result in better spectral deﬁnition (colour saturation). However, increasing thickness re-quires higher operating voltages as it was previously shown in
Fig. 3. Therefore, a trade off between threshold voltage and colour
deﬁnition should be achieved when designing the optimum active layer thickness, depending on the device application requirements.
In this work, several electrical treatments have been performed on diodes with different active layer thickness, based a new
ciano-400 500 600
400 500 600
400 500 600
0.0 0.2 0.4 0.6 0.8 1.0
Normalized EL (a.u.)
Wavelength (nm) J = 40 mA/cm2
0.0 0.2 0.4 0.6 0.8 1.0
Normalized EL (a.u.)
Wavelength (nm) J = 400 mA/cm2
0.0 0.2 0.4 0.6 0.8 1.0
Normalized EL (a.u.)
Wavelength (nm) J = 1400 mA/cm2
0 250 500 750 1000 1250
0.4 0.5 0.6 0.7 0.8
Relative spectral area
Current Density (mA/cm2)
Fig. 10.Normalized EL spectra for a 55 nm sample at different current levels: (a) 40 mA/cm2
, (b) 400 mA/cm2
, and (c) 1400 mA/cm2
. In (d) the sum of the relative defects area is plotted vs. bias current.
400 500 600 700
0.0 5.0x10-6 1.0x10-5 1.5x10-5 2.0x10-5
J = 62 mA/cm2
J = 119 mA/cm2
J = 30 mA/cm2
J = 192 mA/cm2
derivative of the polyﬂuorene–phenylidene, in order to discrimi-nate between different degradation mechanisms. We have re-corded EL, emission and excitation PL spectra to identify and quantify main intrinsic and extrinsic emissive bands, with the aid of spectral energy Gaussian deconvolution.
Our experiments show that the structured band in the 470– 510 nm region arises from a defect, that may be unintentionally enhanced when device layer structure is not optimized. When this structure favours electron accumulation (as a result of having, for example, an electron blocking layer, such as PEDOT:PSS) this band is clearly enhanced during device operation. This effect may be re-duced by increasing the active layer thickness, so that electron accumulation lowers, due to a higher recombination probability along the active layer. The same trend in the ﬂuorenone related de-fect is observed when increasing active layer thickness: thicker samples contain a lower oxygen concentration resulting in a less pronounced peak at 530 nm.
These results lead to a trade off between optical and electrical performance in PLEDs: When designing device layer structure it should be considered that thinner samples result in low threshold voltages but in higher probability of extrinsic peaks in EL spectra.
The authors would like to thank Drs. M. Clement, J. Olivares and F. Calle for thickness measurements. This work was supported in part by Comunidad Autónoma de Madrid under Project S0505/ ESP/000417 and in part by the Spanish Ministry of Education and Science under Projects TEC2006-13392-C02-02/MIC and MAT-2005-1004.
 Bernius MT, Inbasekaran M, O’Brien J, Wu WS. Progress in light emitting polymers. Adv Mater 2000;12:1737–50;
Scherf U, List EJW. Semiconducting polyﬂuorenes. Towards reliable structure– property relationships. Adv Mater 2002;14:477.
 List EJW, Guentner R, de Freitas PS, Scherf U. The effect of keto defect sites on the emission properties of polyﬂuorene-type materials. Adv Mater 2002;14:374–8.
 Montilla F, Pastor I, Mateo CR, Morallón E, Mallavia R. Charge transport in luminescent polymer studied by in situ ﬂuorescence spectroscopy. J Phys Chem B 2006;110:5914–9.
 Bliznyuk VN, Carter SA, Scott JC, Klarner G, Miller RD, Miller DC. Electrical and photoinduced degradation of polyﬂuorene based ﬁlms and light emitting devices. Macromolecules 1999;32:361.
 Sims M, Bradley DDC, Ariu M, Koeberg M, Asimakis A, Grell M, et al. Understanding the origin of the 535 nm emission band in oxidized
Poly(9,9-dioctylﬂuorene): the essential role of inter-chain/inter-segment interactions. Adv Funct Mater 2004;14:765.
 Gaal M, List EJW, Scherf U. Excimer or emissive on–chain defects? Macromolecules 2003;36:1750.
 Romaner L, Pogantsch A, de Freitas PS, Gaal M, Zojer E, List EJW. The origin of green emission in polyﬂuorene-based conjugated polymers: on-chain defect ﬂuorescence. Adv Funct Mater 2003;13:597.
 Zhao W, Cao t, White JM. On the origin of green emission in polyﬂuorene polymers: the roles of thermal oxidation degradation and crosslinking. Adv Funct Mater 2004;14:783.
 Gong XO, Iyer PK, Moses D, Bazan GC, Heeger AJ, Xiao SS. Stabilized blue emission from polyﬂuorene-based light-emitting diodes: elimination of ﬂuorenone defects. Adv Funct Mater 2003;13:325.
 Gammerith S, Nothofer HG, Scherf U, List EJW. Identiﬁcation of emissive interface-related defects in polyﬂuorene based light emitting devices. Jpn J Appl Phys Part 2 2004;42:891.
 Montilla F, Mallavia R. On the origin of green emission bands in ﬂuorene-based conjugated polymers. Adv Funct Mater 2007;17:71.
 Jacob J, Zhang J, Grimsdale AC, Müllen K, Gaal M, List EJW. Poly(tetraarylindenoﬂuorene)s: new stable blue-emitting polymers. Macromolecules 2003;36:8240.
 Ouisse T, Stéphan O, Armand M. Degradation kinetics of the spectral emission in polyﬂuorene light-emitting electro-chemical cells and diodes. Eur Phys J Appl Phys 2003;24:195.
 Chen Zhenyu, Ma D. Improved color purity and efﬁciency in polyﬂuorene-based light emitting diodes. Mater Sci Eng B 2007;141:71–5.
 Mallavia R, Montilla F, Pastor I, Velasquez P, Arredondo B, Alvarez AL, et al. Characterization and side chain manipulation in violet-blue Poly-[(9,9-dialkylﬂuoren-2,7-diyl)-alt-co-(benzen-1,4-diyl) backbones. Macromolecules 2005;38:3185.  Alvarez AL, Arredondo B, Romero B, Gutiérrez-Llorente A, Quintana X, Mallavia
R, et al. Analytical evaluation of the ratio between injection and space-charge limited currents in single carrier organic diodes. IEEE Trans Electron Dev 2008;55(2):674–80.
 Gartner F. A comparison of the electrical properties of polymer LEDs based on poly(thiophene)s and PPV-derivatives. PhD thesis, University of Groningen, The Netherlands, 1997.
 Khan RUA, Bradley DDC, Webster MA, Auld JL, Walker AB. Degradation in blue-emitting conjugated polymer diodes due to loss of ohmic hole injection. Appl Phys Lett 2004;84:921–3.
 Gomes HL, Stallinga P, Cölle M, de Leeuw DM, Biscarini F. Electrical Instabilities in organic semiconductors caused by trapped supercooled water. Appl Phys Lett 2006;88:082101.
 Montilla F, Frutos LM, Mateo CR, Mallavia R. Fluorescence emission anisotropy coupled to an electrochemical system: study of exciton dynamics in conjugated polymers. J Phys Chem C 2007;111:18405.
 Arkhipov VI, Emelianova EV, Tak YH, Bässler H. Charge injection into light-emitting diodes: theory and experiment. J Appl Phys 1998;84:848.  Yan H, Scott BJ, Huang Q, Marks T. Enhanced polymer light-emitting diode
performance using a crosslinked-network electron-blocking interlayer. Adv Mater 2004;16:1948–52.
 Bässler H, tak YH, Khramtchenkov DV, Nikitenko VR. Model sof organic light-emitting diodes. Synth Met 1997;91:173–9.
 Savvate’ev V, Friedl JH, Zou L, Shinar J, Christensen K, Oldham W, et al. Nanosecond electroluminescence spikes from multilayer blue 4,40-bis(2,20
-diphenyl vinyl)-1,10-biphenyl (DPVBi) organic light-emitting devices. Mater
Sci Eng 2001;B85:224–7.